Download presentation

Presentation is loading. Please wait.

Published bySawyer Cates Modified over 2 years ago

1
Phase II Total Fatigue Life (Crack Initiation + Crack Propagation) SAE FD&E Current Effort 30 October 2012 at Peoria, IL

2
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

3
Load Carrying Weld Specimen Configuration and Test Fixture/FEM Boundary Conditions See Next Slide

4
Specimen in Test Rig See Next Slide

5
Specimen Crack After Inability To Carry Load In Test Rig See Next Slide

6
Specimen Crack Fracture Surface Total Prototype Test Fatigue Life (Crack Initiation + Crack Propagation) = 36,895 Cycles

7
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

8
Exact – Same Steel Pedigree (Material Characterization) Definition/Documentation Microstructure, Chemistry & Hardness Sample Purchased “Enough” 4 A36 20ft HR bars

9
Steel Microstructure, Hardness, Grain Size and Chemistry

10
Steel Local Strain Low Cycle Crack Initiation Material Characterization

11
Assumes the welding residual tension stress is equal to the steel’s proportional limit (for Ni analysis only): 1200ue

12
Steel Crack Propagation Material Characterization

13
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

14
Accurate Loading Definition 24 KN to 2.4 KN R=0.1

15
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

16
Component Stress/Strain Distribution Path Across Critical Section

17
Component Stress/Strain Distribution Path At Weld Toe Critical Section FEM Stress FEM Strain

18
Component BS 5400 or BS7608 Stress Analysis (by an expert with decades of experience) and N = 15,500 cycles. Analysis is simple with BS 5400 or BS7608 methods. Input is simply nominal stress range and weld class with a modifier for plate thickness. This is a fillet weld with the stress perpendicular to the toe so I would call it class F. Equation for class F is S=11995(N)^(-0.333) Stress range is = delta m*C/I =.9*24000*225*12.7/(101.6*25.4^3/12)=445 MPa. (This is a bit higher than the 400 I get by extrapolating the linear section of Eric’s plot from FEA.) Since the plate is 1 inch and curves are based on 0.5 strength is modified by (0.5/1)^.25 = 0.84 (This was also proposed by Fred Lawrence.) The intercept of the SN curve would be 11995*0.84 = 10086. Since this is a design curve, I would increase strength by about 10% for this lab test. So 10086*1.1= 11095 and N = 15,500 cycles. Use some judgment in applying this number. Since the R ratio is high, life might be expected to be a bit less but since the calculated elastic stress is above the material strength, there will be yielding so that the actual stress range will likely not be as high as predicted. Also, curves were developed with axial specimens tested to failure and this is bending this piece should last a bit longer. I would expect life to be between 15,000 and 60,000 cycles to get to the point where it will not carry the load.

19
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

20
GeometryLoadingMat’l. Prop. Stress/Strain Analysis Crack Initiation Analysis Program Crack Initiation Life 13,070Cycles Local Strain Low Cycle Crack Initiation Fatigue Analysis Appropriately Meshed Mesh of CAD Geometry 24 KN to 2.4 KN R=0.1 Crack Initiation Material Characterization

21
GeometryLoadingMat’l. Prop. Stress Distribution Crack Propagation Analysis Program Crack Propagation Life 45,190 Cycles Linear Elastic Fracture Mechanics Crack Propagation Fatigue Analysis Appropriately Meshed CAD Geometry 24 KN to 2.4 KN R=0.1 Crack Propagation Material Characterization

22
GeometryLoadingMat’l. Prop. Stress/Strain Analysis Damage Analysis Total Life Total Life = Crack Initiation + Crack Propagation = 13,070 Cycles (CI) + 45,190 Cycles (CP-SE) + 0 Cycles (CP-EC) = 58,260 Cycles Predicted life/Test Life (of 1 Hand Welded Prototype Sample) =58,260 Cycles/36,895 Cycles = 1.6 Total Life

23
Predict the Upper and Lower Total Fatigue Life Bounds (Using “Principal” ue for CI) Loading Direction CI CPCP Free Surface

24
Component BS 5400 or BS7608 Stress Analysis (by an expert with decades of experience) Analysis is simple with BS 5400 or BS7608 methods. Input is simply nominal stress range and weld class with a modifier for plate thickness. This is a fillet weld with the stress perpendicular to the toe so I would call it class F. Equation for class F is S=11995(N)^(-0.333) Stress range is = delta m*C/I =.9*24000*225*12.7/(101.6*25.4^3/12)=445 MPa. (This is a bit higher than the 400 I get by extrapolating the linear section of Eric’s plot from FEA.) Since the plate is 1 inch and curves are based on 0.5 strength is modified by (0.5/1)^.25 = 0.84 (This was also proposed by Fred Lawrence.) The intercept of the SN curve would be 11995*0.84 = 10086. Since this is a design curve, I would increase strength by about 10% for this lab test. So 10086*1.1= 11095 and N = 15,500 cycles. Use some judgment in applying this number. Since the R ratio is high, life might be expected to be a bit less but since the calculated elastic stress is above the material strength, there will be yielding so that the actual stress range will likely not be as high as predicted. Also, curves were developed with axial specimens tested to failure and this is bending this piece should last a bit longer. I would expect life to be between 15,000 and 60,000 cycles to get to the point where it will not carry the load.

25
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

26
0.200 in 1.467 in 0.312 in holes Accurate Scanning Electron Microscope (SEM) Crack Growth Measurements a a To be evaluated by a second robotic welded prototype test R = 0.5

27
Effort Definition 1)Steel procurement, prototype test specimen design/fabrication, prototype test and prototype test result. 2)Steel pedigree (material characterization) definition/documentation. 3)Accurate loading definition 4)Test component geometry for stress/strain (FEM and other) analysis. 5)Total fatigue life predictions (crack initiation + crack propagation and other). 6)The next (crucial) step for discerning the transition from crack initiation to crack propagation. 7)Test Matrix and Future Work (committed to and not committed to).

28
Test Matrix and Future Work : Read marker band “striation patterns

29
Machined Specimen Configuration and Test Fixture/FEM Boundary Conditions Eliminate the weld entirely – machine the entire specimen from the 101.6 mm x 101.6 mm bar. Duplicate, by machining, the weld profile and weld toe radius as closely as possible so the sample is consistently made from the same material. Comparing the test results from these samples relative to the test results from the previously welded samples. This will confirm (or not) how sound an assumption it is to use the base material properties when analyzing welded structures.

Similar presentations

OK

Mechanics of Elastic Materials. Why study mechanics? Useful for the analysis and design of load-bearing structures, such as: buildings bridges space shuttles.

Mechanics of Elastic Materials. Why study mechanics? Useful for the analysis and design of load-bearing structures, such as: buildings bridges space shuttles.

© 2018 SlidePlayer.com Inc.

All rights reserved.

Ads by Google

Ppt on wastage of time energy and money Ppt on surface water tension Ppt on travel and tourism in india free download Ppt on low level language vs high level Ppt on library management system free download Ppt on adivasis of india Download ppt on oxidation and reduction in chemistry View my ppt online templates Ppt on bluetooth communication ios Ppt on community health and environment